Macromolecules 2000, 33, 6310-6314
Synthesis of Polymethyl(trimethylsiloxy)siloxane by Anionic Ring-Opening Polymerization of 1,3,5-Trimethyl-1,3,5-tris(trimethylsiloxy)cyclotrisiloxane Guo Ping Cai and William P. Weber* D. P. and K. B. Loker Hydrocarbon Research Institute, Department of Chemistry, University of Southern California, Los Angeles, California 90089-1661 Received March 3, 2000; Revised Manuscript Received June 20, 2000
ABSTRACT: Polymethyl(trimethylsiloxy)siloxane, the first linear polysiloxane in which each silicon atom of the polymer backbone is a trifunctional RSiO3/2 (T) unit, has been prepared by anionic ring-opening polymerization of 1,3,5-trimethyl-1,3,5-tris(trimethylsiloxy)cyclotrisiloxane (I).
Introduction Soluble linear polysiloxanes are commercially the most important type of inorganic/organic polymeric material. The backbone of these is generally made up of difunctional R2SiO2/2 (D) units in which R is typically methyl, phenyl, 3,3,3-trifluoropropyl, 3-cyanopropyl, or H.1 Polydisperse high molecular weight linear polysiloxanes are often prepared by acid-catalyzed ringopening polymerization of cyclotetrasiloxanes such as octamethylcyclotetrasiloxane (D4).2,3 Small amounts of a disiloxane, such as hexamethyldisiloxane (MM) which can serve as an end-capping unit, permit control of the molecular weight of the polymer. 2 Trifunctional RSiO3/2 (T) units are found at branch points or cross-links. Linear polysiloxane in which T units serve as the polymer backbone have not been previously reported. Living anionic ring-opening polymerization of cyclotrisiloxane has been used to prepare narrow molecular weight distribution polysiloxanes.4,5 This is possible because ring opening is generally faster than equilibration or redistribution reactions. Regiospecific anionic ring-opening polymerization of monosubstituted cyclotrisiloxanes has been used to prepare highly regular polysiloxanes.6,7 Results Polymethyl(trimethylsiloxy)siloxane, a linear polymer in which each siloxane unit of the polymer chain is a T unit, has been prepared by anionic ring-opening polymerization of I initiated by dilithiodiphenylsilanediolate (Figure 1).4 I was previously prepared in very low yield by hydrolytic polycondensation of methyltrichlorosilane with sodium metasilicate followed by trimethylsilylation with trimethylchlorosilane.8 We have prepared I by reaction of 1,1-dichlorotetramethyldisiloxane (II)9,10 with DMSO.11-14 Alternatively, I has been prepared by reaction of II with 1,3-dihydroxy-1,3-dimethyl-1,3-bis(trimethylsiloxy)disiloxane (III)15 in the presence of triethylamine. III was prepared by a palladium-oncarbon catalyzed oxidation of 1,3-dihydrido-1,3-dimethyl-1,3-bis(trimethylsiloxy)disiloxane with water.16 III is expected to be inherently unstable since silanols * Corresponding author. e-mail: [email protected]
are well-known to undergo facile condensation to siloxanes. For this reason, III was reacted with II promptly after its preparation. Both methods to prepare I require II, which is not commercially available. We have prepared II by the ferric chloride/HCl superacid (HFeCl4) catalyzed equilibration of hexamethyldisiloxane and methyltrichlorosilane.17 In this reaction, trimethylchlorosilane is lost. In addition to II, a small amount of methylbis(trimethylsiloxy)chlorosilane is formed. II has previously been prepared by equilibration of methyltrichlorosilane and hexamethyldisiloxane in the presence of cyclic (PNCl2)n (Figure 2).9 Although I, II, and III have been previously reported, they have not been fully characterized by modern spectroscopic methods. For this reason, we have included full experimental details and spectral characterization. Experimental Section 1H, 13C, and 29Si NMR spectra were obtained on a Bruker AMX-500 MHz spectrometer. 13C NMR spectra were obtained with broad-band proton decoupling. Spectra of monomers were run in acetone-d6. Because of its limited solubility in acetone, spectra of polymethyl(trimethylsiloxy)siloxane were run in benzene-d6. 1H and 13C NMR spectra were internally referenced to residual acetone. A heteronuclear gated decoupling pulse sequence (NONOE) with a 60 s delay (for monomers) and a 30 s delay (for polymers) was used to acquire the 29Si NMR spectra. These were referenced to an external TMS standard. IR spectra of neat films on NaCl plates for liquids were recorded on a Perkin-Elmer Spectrum 2000 FT-IR spectrometer. GPC analysis of the molecular weight distribution of the polymers was performed at 22 °C on a Waters system equipped with a R401 refractive index detector. Two 7.8 mm × 300 mm Styragel columns packed with